Self-assembled monolayer of designed and synthesized triazinedithiolsilane molecule as interfacial adhesion enhancer for integrated circuit
© Wang et al; licensee Springer. 2011
Received: 10 May 2011
Accepted: 3 August 2011
Published: 3 August 2011
Self-assembled monolayer (SAM) with tunable surface chemistry and smooth surface provides an approach to adhesion improvement and suppressing deleterious chemical interactions. Here, we demonstrate the SAM comprising of designed and synthesized 6-(3-triethoxysilylpropyl)amino-1,3,5-triazine-2,4-dithiol molecule, which can enhance interfacial adhesion to inhibit copper diffusion used in device metallization. The formation of the triazinedithiolsilane SAM is confirmed by X-ray photoelectron spectroscopy. The adhesion strength between SAM-coated substrate and electroless deposition copper film was up to 13.8 MPa. The design strategy of triazinedithiolsilane molecule is expected to open up the possibilities for replacing traditional organosilane to be applied in microelectronic industry.
Isolating individual components of nanoscale architectures comprised of thin films or nanostructures is a critical challenge in micro- and nanoscale device fabrication . One important example that illustrates this challenge could be seen in Cu-interconnected sub-100-nm device structures, which require less than 5-nm-thick interfacial layers to inhibit Cu diffusion into adjacent dielectrics . Conventional interfacial barrier layers such as TaN, Ta, Ti, TiN, or W have already been optimized in microelectronic applications. However, such "thick" layers are not suitable for micro- and nanoscale device fabrication, and the above materials cannot form uniform and continuous film below 5 nm in thickness . The barrier layer thickness must be minimized while maintaining high-performance diffusion barrier properties and good adhesion strength with neighboring layers . Another significant example is seen in the adhesion between copper and substrate in printed circuit board technology.
An alternative to the above interfacial layer is the organic self-assembled monolayer (SAM)  with sub-nanometer dimensions. The SAM [6, 7] composed of short aliphatic chains with desired terminal function groups has been investigated by modifying surface properties for the above requirement. The selectivity and adhesion strength between the function group of SAM and the substrate impact the film packing density and thermal stability, and the chain length also has influence on the packing density and order. In recent years, G. Ramanath has reported the technique of fabricating SAM with the organosilanes as Cu diffusion barrier layer, and interfacial adhesion in microelectronics devices [2, 8–12]. The results showed that the SAM inhibited Cu diffusion into substrate interface and enhanced the interfacial adhesion to increase the device lifetime [8, 13]. This technique has two advantages: (a) a strong interfacial bonding which can immobilize Cu, and (b) the creation of a vacuum-like potential barrier between Cu and the dielectric layer to inhibit Cu ionization and transport . The former can be achieved through strong, local chemical interaction by choosing appropriate terminal groups, and the latter can be accomplished by using SAM with suitable chain length or the introduction of aromatic group. This technique offers the potential for tailoring effective barriers with decreased thickness.
Chemical formula and nomenclature of the self-assembled organosilanes usually used in previous researches
From the results of Table 1, we can learn that the mercapto-silane (SAM1), amino-silane (SAM2 ), and pyridyl-silane (SAM4) are excellent coupling agents between substrates and Cu to act as interfacial adhesion enhancer. Compared with aliphatic groups, larger volume organosilanes with the aromatic ring (SAM4, SAM5, SAM6, and SAM7 ) sterically hinder copper diffusion. Therefore, the ideal organosilane molecules should be with both aromatic ring and terminal function group which have high reactivity with copper. In recent years, studies have been mainly focused on the approaches of Cu metallization including chemical vapor deposition, physical vapor deposition, electroless deposition (ELD), and electroplating. Cu ELD was especially emphasized in future interconnect technology. However, the organosilanes utilized in this technique were mainly mercaptopropyltrimethoxysilane (MPTMS; SAM1 [3, 9–11]) and aminopropyltrimethoxysilane (APTMS; SAM2 [4, 9, 17]). So far, no research has been carried out on the modification of organosilane, and it is necessary to design and synthesize functional organosilane molecule.
In this paper, we demonstrate a designed and synthesized triazinedithiolsilane molecule - 6-(3-triethoxysilylpropyl)amino-1,3,5-triazine-2,4-dithiol monosodium salt (abbreviation, TESPA, see Figure 1) according to the strategies mentioned. TESPA has three active sites which refer to two mercapto groups  and a nitrogen atom. We also preliminarily investigate the adhesion strength between ELD copper film and TESPA SAM to verify whether it can be used as adhesion enhancer and diffusion barrier in device applications.
The chemical structure of TESPA was identified by nuclear magnetic resonance (NMR), Fourier transform infrared spectroscopy (FT-IR), and mass spectroscopy (MS) (The data are available in Additional file 1). 1H NMR and 13C NMR spectra were recorded by Bruker AC 400 with 500 MHz (Bruker Daltonics, Billerica, MA, USA). FT-IR spectra were measured using Bruker TENSOR 37 (Bruker Daltonics). MS was recorded by LCQ-Fleet (Thermo Scientific, Waltham, MA, USA).
TESPA SAM was fabricated on epoxy resin surface. The epoxy resin surface was treated by corona discharge for 10 s to facilitate the formation of SAM through surface hydroxylation. TESPA SAM was obtained by dipping the epoxy resin into 2.5 mM TESPA monomer ethanol-water (V/V = 95:5) solution for 5 min at room temperature. The substrate was dried with nitrogen gas and cured at 120°C for 20 min. Then, a Sn-PdII colloidal solution was used as a catalyst precursor , which was prepared via precise control of sequential hydrolysis of PdII species according to the hydrolysis mechanism of PdII salts in a chloride-rich aqueous solution. The electroless deposition bath was prepared according to recent study . X-ray photoelectron spectroscopy (XPS) was performed to investigate the elemental composition of surface by using ULVAC PHI-5600 spectrometer (Ulvac Technologies, Inc., Methuen, MA, USA). The adhesion strength between ELD copper film and TESPA SAM-coated epoxy resin substrate was investigated by T-peel test using an autograph S-100 apparatus (Shimadzu Corporation, Kyoto, Japan).
Results and discussion
TESPA was synthesized by the reaction of cyanuric chloride, 3-aminopropyltriethoxy silane (APTES), and NaSH according to the strategy described in the Figure 1. The stirring tetrahydrofuran (THF) solution of cyanuric chloride (0.1 mol) was added with APTES (0.1 mol) over a period of 60 min. And then the reaction mixture was added with THF solution of triethylamine (0.12 mol) for 1-day reaction. After, the solvent was removed under vacuum to yield 6-(3-triethoxysilylpropyl)amino-1,3,5-triazine-2,4-dichloride. NaSH ethanol solution was added dropwise for 2-h reaction to the ethanol solution of the dichloride. After, the solvent was removed under vacuum to yield TESPA. Yield was 75.6%, and m.p. > 203°C. Elemental analysis calculation for C12H23N4S2O3NaSi was: C, 37.29%; H, 6.00%; N, 14.49%; however, found was: C, 37.46%; H, 6.03%; and N, 14.44%. The results of NMR, FT-IR, and MS also suggest that TESPA have been synthesized (see Additional file 1).
The functional triazinedithiolsilane molecule TESPA was designed and synthesized. The Si-OH group of hydrolyzed TESPA could react with the polar groups on pretreated epoxy resin surface to form the TESPA SAM, which promote ELD copper film onto the substrate. The adhesion strength between TESPA SAM-coated epoxy resin and ELD copper film was up to 13.8 MPa, which could satisfy the purpose of TESPA SAM applied as adhesion enhancer. The design strategy of TESPA will provide possibilities for replacing the traditional organosilane (MPTMS, APTMS, etc.) to be applied in microelectronic industry.
The authors express their sincere gratitude for the financial support of the Scientific Research Foundation for the Returned Overseas Chinese Scholars, State Education Ministry (no. K314020902) and the Fundamental Research Funds for the Central Universities (no. Z109021008).
- Kuech TF, Mawst LJ: Nanofabrication of III-V semiconductors employing diblock copolymer lithography. J Phys D: Appl Phys 2010, 43: 183001. 10.1088/0022-3727/43/18/183001View ArticleGoogle Scholar
- Gandhi D, Lane M, Zhou Y, Singh A, Nayak S, Tisch U, Eizenberg M, Ramanath G: Annealing-induced interfacial toughening using a molecular nanolayer. Nature 2007, 447: 299. 10.1038/nature05826View ArticleGoogle Scholar
- Doppelt P, Semaltianos N, Deville Cavellin C, Pastol J, Ballutaud D: High affinity self-assembled monolayers for copper CVD. Microelectron Eng 2004, 76: 113. 10.1016/j.mee.2004.07.023View ArticleGoogle Scholar
- Caro A, Armini S, Richard O, Maes G, Borghs G, Whelan C, Travaly Y: Bottom-up engineering of subnanometer copper diffusion barriers using NH 2 -derived self-assembled monolayers. Adv Funct Mater 2010, 20: 1125. 10.1002/adfm.200902072View ArticleGoogle Scholar
- Liu G, Zhao H, Zhang J, Park JH, Mawst LJ, Tansu N: Selective area epitaxy of ultra-high density InGaN quantum dots by diblock copolymer. Nanoscale Res Lett 2011, 6: 342. 10.1186/1556-276X-6-342View ArticleGoogle Scholar
- Moores B, Simons J, Xu S, Leonenko Z: AFM-assisted fabrication of thiol SAM pattern with alternating quantified surface potential. Nanoscale Res Lett 2011, 6: 185. 10.1186/1556-276X-6-185View ArticleGoogle Scholar
- Demirel G, Caglayan MO, Garipcan B, Duman M, Piskin E: Formation and organization of amino terminated self-assembled layers on Si(001) surface. Nanoscale Res Lett 2007, 2: 350. 10.1007/s11671-007-9071-7View ArticleGoogle Scholar
- Krishnamoorthy A, Chanda K, Murarka S, Ramanath G, Ryan J: Self-assembled near-zero-thickness molecular layers as diffusion barriers for Cu metallization. Appl Phys Lett 2001, 78: 2467. 10.1063/1.1365418View ArticleGoogle Scholar
- Gandhi D, Ganesan P, Chandrasekar V, Gan Z, Mhaisalkar S, Li H, Ramanath G: Molecular-nanolayer-induced suppression of in-plane Cu transport at Cu-silica interfaces. Appl Phys Lett 2007, 90: 163507. 10.1063/1.2722667View ArticleGoogle Scholar
- Gandhi D, Tisch U, Singh B, Eizenberg M, Ramanath G: Ultraviolet-oxidized mercaptan-terminated organosilane nanolayers as diffusion barriers at Cu-silica interfaces. Appl Phys Lett 2007, 91: 143503. 10.1063/1.2760164View ArticleGoogle Scholar
- Ganesan P, Kumar A, Ramanath G: Surface oxide reduction and bilayer molecular assembly of a thiol-terminated organosilane on Cu. Appl Phys Lett 2005, 87: 011905. 10.1063/1.1968414View ArticleGoogle Scholar
- Garg S, Singh B, Teki R, Lane M, Ramanath G: Hydrophobic fluoroalkylsilane nanolayers for inhibiting copper diffusion into silica. Appl Phys Lett 2010, 96: 143121. 10.1063/1.3374453View ArticleGoogle Scholar
- Hu M, Noda S, Tsuji Y, Okubo T, Yamaguchi Y, Komiyama H: Effect of interfacial interactions on the initial growth of Cu on clean SiO2 and 3-mercaptopropyltrimethoxysilane-modified SiO2 substrates. J Vac Sci Technol A 2002, 20: 589. 10.1116/1.1458941View ArticleGoogle Scholar
- McBrayer J, Swanson R, Sigmon T: Diffusion of metals in silicon dioxide. J Electrochem Soc 1986, 133: 1242. 10.1149/1.2108827View ArticleGoogle Scholar
- Ganesan P, Singh A, Ramanath G: Diffusion barrier properties of carboxyl-and amine-terminated molecular nanolayers. Appl Phys Lett 2004, 85: 579. 10.1063/1.1775035View ArticleGoogle Scholar
- Mikami N, Hata N, Kikkawa T, Machida H: Robust self-assembled monolayer as diffusion barrier for copper metallization. Appl Phys Lett 2003, 83: 5181. 10.1063/1.1635665View ArticleGoogle Scholar
- Rebiscoul D, Perrut V, Morel T, Jayet C, Cubitt R, Haumesser P: Alkoxysilane layers compatible with copper deposition for advanced semiconductor device applications. Langmuir 2010, 26: 8981. 10.1021/la904771sView ArticleGoogle Scholar
- Wang F, Wang Y, Li Y, Wang Q: Preparation of triazinedithiol polymeric nanofilm by two-step potentiostatic polymerization technique on aluminum surface. Mater Lett 2010, 65: 621.View ArticleGoogle Scholar
- Wang F, Mori K, Kang Z, Oishi Y: Magnetic field effects on the polymerization of 6- N, N -dioctylamino-1,3,5-triazine-2,4-dithiol. Heteroat Chem 2007, 18: 60. 10.1002/hc.20257View ArticleGoogle Scholar
- Mori K, Suzuki K, Shimizu K, Oishi Y: Evaporation polymerization of 6-dibutylamino-1,3,5-triazine-2,4-dithiol on iron plates. Langmuir 2002, 18: 9527. 10.1021/la020301hView ArticleGoogle Scholar
- Rezaee A, Pavelka LC, Mittler S: Binary mixtures of SH- and CH3-terminated self-assembled monolayers to control the average spacing between aligned gold nanoparticles. Nanoscale Res Lett 2009, 4: 1319. 10.1007/s11671-009-9399-2View ArticleGoogle Scholar
- Brandow S, Chen M, Aggarwal R, Dulcey C, Calvert J, Dressick W: Fabrication of patterned amine reactivity templates using 4-chloromethylphenylsiloxane self-assembled monolayer films. Langmuir 1999, 15: 5429. 10.1021/la9902082View ArticleGoogle Scholar
- Fujiwara Y, Kobayashi Y, Sugaya T, Koishikawa A, Hoshiyama Y, Miyake H: Adsorption promotion of Ag nanoparticle using cationic surfactants and polyelectrolytes for electroless Cu plating catalysts. J Electrochem Soc 2010, 157: D211. 10.1149/1.3306025View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.